Download presentation

Presentation is loading. Please wait.

1
**Chapter 6 – Mechanical Properties and Behavior**

The Science and Engineering of Materials, 4th ed Donald R. Askeland – Pradeep P. Phulé Chapter 6 – Mechanical Properties and Behavior

2
Objectives of Chapter 6 Introduce the basic concepts associated with mechanical properties of materials. Evaluate factors that affect the mechanical properties of materials. Review some of the basic testing procedures that engineers use to evaluate many of these properties.

3
**Chapter Outline 6.1 Technological Significance**

6.2 Terminology for Mechanical Properties 6.3 The Tensile Test: Use of the Stress-Strain Diagram 6.4 Properties Obtained from the Tensile Test 6.5 True Stress and True Strain 6.6 The Bend Test for Brittle Materials 6.7 Hardness of Materials 6.8 Strain Rate Effects and Impact Behavior 6.9 Properties Obtained from the Impact Test 6.10 Fracture Mechanics 6.11 The Importance of Fracture Mechanics

4
**Chapter Outline(Continued)**

6.12 Microstructural Features of Fracture in Metallic Materials 6.13 Microstructural Features of Fracture in Ceramics, Glasses, and Composites 6.14 Weibull Statistics for Failure Strength Analysis 6.15 Fatigue 6.16 Results of the Fatigue Test 6.17 Application of Fatigue Testing 6.18 Creep, Stress Rupture, and Stress Corrosion 6.19 Evaluation of Creep Behavior 6.20 Use of Creep Data 6.21 Superplasticity

5
**Section 6.1 Technological Significance**

Figure 6.1 Aircraft, such as the one shown here, makes use of aluminum alloys and carbon-fiber-reinforced composites. (Courtesy of Getty Images.) Figure 6.2 The materials used in sports equipment must be lightweight, stiff, tough, and impact resistant. (Courtesy of Getty Images.)

6
**Section 6.2 Terminology for Mechanical Properties**

Stress - Force or load per unit area of cross-section over which the force or load is acting. Strain - Elongation change in dimension per unit length. Young’s modulus - The slope of the linear part of the stress-strain curve in the elastic region, same as modulus of elasticity. Shear modulus (G) - The slope of the linear part of the shear stress-shear strain curve. Viscosity ( ) - Measure of resistance to flow, defined as the ratio of shear stress to shear strain rate (units Poise or Pa-s). Thixotropic behavior - Materials that show shear thinning and also an apparent viscosity that at a constant rate of shear decreases with time.

7
**(c)2003 Brooks/Cole, a division of Thomson Learning, Inc**

(c)2003 Brooks/Cole, a division of Thomson Learning, Inc. Thomson Learning™ is a trademark used herein under license. Figure 6.3 (a) Tensile, compressive, shear and bending stresses. (b) Illustration showing how Young’s modulus is defined for elastic material. (c) For nonlinear materials, we use the slope of a tangent as a variable quantity that replaces the Young’s modulus constant

8
**Figure 6. 4 (a) Various types of strain response to an imposed stress**

Figure 6.4 (a) Various types of strain response to an imposed stress. (Source: Reprinted from Materials Principles and Practice, by C. Newey and G. Weaver (Eds.), 1991 p. 300, Fig Copyright © 1991 Butterworth-Heinemann. Reprinted with permission from Elsevier Science.)

9
Figure 6.4 (Continued) (a) Various types of strain response to an imposed stress. (Source: Reprinted from Materials Principles and Practice, by C. Newey and G. Weaver (Eds.), 1991 p. 300, Fig Copyright © 1991 Butterworth-Heinemann. Reprinted with permission from Elsevier Science.) (b) Stress relaxation in a viscoelastic material. Note the y-axis is stress. Strain is constant.

10
**(c)2003 Brooks/Cole, a division of Thomson Learning, Inc**

(c)2003 Brooks/Cole, a division of Thomson Learning, Inc. Thomson Learning™ is a trademark used herein under license. Figure 6.5 Shear stress strain rate relationships for Newtonian and non-Newtonian materials

11
**(c)2003 Brooks/Cole, a division of Thomson Learning, Inc**

(c)2003 Brooks/Cole, a division of Thomson Learning, Inc. Thomson Learning™ is a trademark used herein under license. Figure 6.6 (a) Apparent viscosity as a function of shear log (shear rate ) strain rate. (b) and (c) illustration of a Bingham plastic (Equations 6-3a & b). Note the x-axis on (b) is shear strain .

12
**Section 6.3 The Tensile Test: Use of the Stress-Strain Diagram**

Load - The force applied to a material during testing. Strain gage or Extensometer - A device used for measuring change in length and hence strain. Glass temperature (Tg ) - A temperature below which an otherwise ductile material behaves as if it is brittle. Engineering stress - The applied load, or force, divided by the original cross-sectional area of the material. Engineering strain - The amount that a material deforms per unit length in a tensile test.

13
**(c)2003 Brooks/Cole, a division of Thomson Learning, Inc**

(c)2003 Brooks/Cole, a division of Thomson Learning, Inc. Thomson Learning™ is a trademark used herein under license. Figure 6.7 A unidirectional force is applied to a specimen in the tensile test by means of the moveable crosshead. The cross-head movement can be performed using screws or a hydraulic mechanism

14
**(c)2003 Brooks/Cole, a division of Thomson Learning, Inc**

(c)2003 Brooks/Cole, a division of Thomson Learning, Inc. Thomson Learning™ is a trademark used herein under license. Figure 6.9 Tensile stress-strain curves for different materials. Note that these are qualitative

16
**(c)2003 Brooks/Cole, a division of Thomson Learning, Inc**

(c)2003 Brooks/Cole, a division of Thomson Learning, Inc. Thomson Learning™ is a trademark used herein under license. Figure The stress-strain curve for an aluminum alloy from Table 6-1

17
**Tensile Testing of Aluminum Alloy**

Example 6.1 Tensile Testing of Aluminum Alloy Convert the change in length data in Table 6-1 to engineering stress and strain and plot a stress-strain curve.

18
Example 6.1 SOLUTION

20
**Design of a Suspension Rod**

Example 6.2 Design of a Suspension Rod An aluminum rod is to withstand an applied force of 45,000 pounds. To assure a sufficient safety, the maximum allowable stress on the rod is limited to 25,000 psi. The rod must be at least 150 in. long but must deform elastically no more than 0.25 in. when the force is applied. Design an appropriate rod. Example 6.2 SOLUTION

21
**Example 6.2 SOLUTION(Continued)**

22
**Section 6.4 Properties Obtained from the Tensile Test**

Elastic limit Tensile strength, Necking Hooke’s law Poisson’s ratio Modulus of resilience (Er) Tensile toughness Ductility

23
**(c)2003 Brooks/Cole, a division of Thomson Learning, Inc**

(c)2003 Brooks/Cole, a division of Thomson Learning, Inc. Thomson Learning™ is a trademark used herein under license. Figure (a) Determining the 0.2% offset yield strength in gray cast ion, and (b) upper and lower yield point behavior in a low-carbon steel

24
**(c)2003 Brooks/Cole, a division of Thomson Learning, Inc**

(c)2003 Brooks/Cole, a division of Thomson Learning, Inc. Thomson Learning™ is a trademark used herein under license. Figure Localized deformation of a ductile material during a tensile test produces a necked region. The micrograph shows necked region in a fractured sample

25
Figure 6.13 Typical yield strength values for different engineered materials. (Source: Reprinted from Engineering Materials I, Second Edition, M.F. Ashby and D.R.H. Jones, 1996, Fig. 8-12, p. 85. Copyright © Butterworth-Heinemann. Reprinted with permission from Elsevier Science.)

27
**(c)2003 Brooks/Cole, a division of Thomson Learning, Inc**

(c)2003 Brooks/Cole, a division of Thomson Learning, Inc. Thomson Learning™ is a trademark used herein under license. Figure Comparison of the elastic behavior of steel and aluminum. For a given stress, aluminum deforms elastically three times as much as does steel

28
Figure 6.15 Range of elastic moduli for different engineered materials. (Source: Reprinted from Engineering Materials I, Second Edition, M.F. Ashby and D.R.H. Jones, 1996, Fig. 3-5, p. 35, Copyright © 1996 Butterworth-Heinemann. Reprinted with permission from Elsevier Science.)

29
**Example 6.3 Young’s Modulus of Aluminum Alloy**

From the data in Example 6.1, calculate the modulus of elasticity of the aluminum alloy. Use the modulus to determine the length after deformation of a bar of initial length of 50 in. Assume that a level of stress of 30,000 psi is applied. Example 6.3 SOLUTION

30
**Example 6.4 Ductility of an Aluminum Alloy**

The aluminum alloy in Example 6.1 has a final length after failure of in. and a final diameter of in. at the fractured surface. Calculate the ductility of this alloy. Example 6.4 SOLUTION

31
**(c)2003 Brooks/Cole, a division of Thomson Learning, Inc**

(c)2003 Brooks/Cole, a division of Thomson Learning, Inc. Thomson Learning™ is a trademark used herein under license. Figure The effect of temperance (a) on the stress-strain curve and (b) on the tensile properties of an aluminum alloy

32
**Section 6.5 True Stress and True Strain**

True stress The load divided by the actual cross-sectional area of the specimen at that load. True strain The strain calculated using actual and not original dimensions, given by εt ln(l/l0). (c)2003 Brooks/Cole, a division of Thomson Learning, Inc. Thomson Learning™ is a trademark used herein under license. Figure The relation between the true stress-true strain diagram and engineering stress-engineering strain diagram. The curves are identical to the yield point

33
**Example 6.5 True Stress and True Strain Calculation**

Compare engineering stress and strain with true stress and strain for the aluminum alloy in Example 6.1 at (a) the maximum load and (b) fracture. The diameter at maximum load is in. and at fracture is in. Example 6.5 SOLUTION

34
**Example 6.5 SOLUTION (Continued)**

35
**Section 6.6 The Bend Test for Brittle Materials**

Bend test - Application of a force to the center of a bar that is supported on each end to determine the resistance of the material to a static or slowly applied load. Flexural strength or modulus of rupture -The stress required to fracture a specimen in a bend test. Flexural modulus - The modulus of elasticity calculated from the results of a bend test, giving the slope of the stress-deflection curve.

36
**(c)2003 Brooks/Cole, a division of Thomson Learning, Inc**

(c)2003 Brooks/Cole, a division of Thomson Learning, Inc. Thomson Learning™ is a trademark used herein under license. Figure The stress-strain behavior of brittle materials compared with that of more ductile materials

37
**(c)2003 Brooks/Cole, a division of Thomson Learning, Inc**

(c)2003 Brooks/Cole, a division of Thomson Learning, Inc. Thomson Learning™ is a trademark used herein under license. Figure (a) The bend test often used for measuring the strength of brittle materials, and (b) the deflection δ obtained by bending

38
**Figure 6.20 Stress-deflection curve for Mg0 obtained from a bend test**

(c)2003 Brooks/Cole, a division of Thomson Learning, Inc. Thomson Learning™ is a trademark used herein under license. Figure Stress-deflection curve for Mg0 obtained from a bend test

39
**Figure 6.21 (a) Three point and (b) four-point bend test setup**

(c)2003 Brooks/Cole, a division of Thomson Learning, Inc. Thomson Learning™ is a trademark used herein under license. Figure (a) Three point and (b) four-point bend test setup

41
**Example 6.6 Flexural Strength of Composite Materials**

The flexural strength of a composite material reinforced with glass fibers is 45,000 psi and the flexural modulus is 18 106 psi. A sample, which is 0.5 in. wide, in. high, and 8 in. long, is supported between two rods 5 in. apart. Determine the force required to fracture the material and the deflection of the sample at fracture, assuming that no plastic deformation occurs. Example 6.6 SOLUTION

42
**Example 6.6 SOLUTION (Continued)**

43
**Section 6.7 Hardness of Materials**

Hardness test - Measures the resistance of a material to penetration by a sharp object. Macrohardness - Overall bulk hardness of materials measured using loads >2 N. Microhardness Hardness of materials typically measured using loads less than 2 N using such test as Knoop (HK). Nano-hardness - Hardness of materials measured at 1–10 nm length scale using extremely small (~100 µN) forces.

44
**Figure 6.23 Indentors for the Brinell and Rockwell hardness tests**

(c)2003 Brooks/Cole, a division of Thomson Learning, Inc. Thomson Learning™ is a trademark used herein under license. Figure Indentors for the Brinell and Rockwell hardness tests

46
**Section 6.8 Strain Rate Effects and Impact Behavior**

Impact test - Measures the ability of a material to absorb the sudden application of a load without breaking. Impact energy - The energy required to fracture a standard specimen when the load is applied suddenly. Impact toughness - Energy absorbed by a material, usually notched, during fracture, under the conditions of impact test. Fracture toughness - The resistance of a material to failure in the presence of a flaw.

47
**(c)2003 Brooks/Cole, a division of Thomson Learning, Inc**

(c)2003 Brooks/Cole, a division of Thomson Learning, Inc. Thomson Learning™ is a trademark used herein under license. Figure The impact test: (a) The Charpy and Izod tests, and (b) dimensions of typical specimens

48
**Section 6.9 Properties Obtained from the Impact Test**

Ductile to brittle transition temperature (DBTT) - The temperature below which a material behaves in a brittle manner in an impact test. Notch sensitivity - Measures the effect of a notch, scratch, or other imperfection on a material’s properties, such as toughness or fatigue life.

49
**(c)2003 Brooks/Cole, a division of Thomson Learning, Inc**

(c)2003 Brooks/Cole, a division of Thomson Learning, Inc. Thomson Learning™ is a trademark used herein under license. Figure Results from a series of Izod impact tests for a super-tough nylon thermoplastic polymer

50
**(c)2003 Brooks/Cole, a division of Thomson Learning, Inc**

(c)2003 Brooks/Cole, a division of Thomson Learning, Inc. Thomson Learning™ is a trademark used herein under license. Figure The Charpy V-notch properties for a BCC carbon steel and a FCC stainless steel. The FCC crystal structure typically leads top higher absorbed energies and no transition temperature

51
**(c)2003 Brooks/Cole, a division of Thomson Learning, Inc**

(c)2003 Brooks/Cole, a division of Thomson Learning, Inc. Thomson Learning™ is a trademark used herein under license. Figure The area contained within the true stress-true strain curve is related to the tensile toughness. Although material B has a lower yield strength, it absorbs a greater energy than material A. The energies from these curves may not be the same as those obtained from impact test data

52
**Example 6.7 Design of a Sledgehammer**

The flexural strength of a composite material reinforced with glass fibers is 45,000 psi and the flexural modulus is 18 106 psi. A sample, which is 0.5 in. wide, in. high, and 8 in. long, is supported between two rods 5 in. apart. Determine the force required to fracture the material and the deflection of the sample at fracture, assuming that no plastic deformation occurs. Example 6.7 SOLUTION Design requirements to be met by the sledgehammer. A partial list: 1. The handle should be light in weight, yet tough enough that it will not catastrophically break. 2. The head must not break or chip during use, even in subzero temperatures. 3. The head must not deform during continued use. 4. The head must be large enough to assure that the user doesn’t miss the fence post, and it should not include sharp notches that might cause chipping. 5. The sledgehammer should be inexpensive.

53
**Section 6.10 Fracture Mechanics**

Fracture mechanics - The study of a material’s ability to withstand stress in the presence of a flaw. Fracture toughness - The resistance of a material to failure in the presence of a flaw.

54
**(c)2003 Brooks/Cole, a division of Thomson Learning, Inc**

(c)2003 Brooks/Cole, a division of Thomson Learning, Inc. Thomson Learning™ is a trademark used herein under license. Figure Schematic drawing of fracture toughness specimens with (a) edge and (b) internal flaws

55
**(c)2003 Brooks/Cole, a division of Thomson Learning, Inc**

(c)2003 Brooks/Cole, a division of Thomson Learning, Inc. Thomson Learning™ is a trademark used herein under license. Figure The fracture toughness Kc of a 3000,000psi yield strength steel decreases with increasing thickness, eventually leveling off at the plane strain fracture toughness Klc

57
Figure 6-33 A scanning electron micrograph showing crack propagation in a PZT ceramic. (Courtesy of Wang and Raj N. Singh, Ferroelectrics, 207, 555–575 (1998).) Figure 6-32 Secondary cracks developed during hardness testing can be used to assess the fracture toughness of brittle materials

58
Figure 6-34 Fracture toughness versus strength of different engineered materials. (Source: Adapted from Mechanical Behavior of Materials, by T.H. Courtney, 2000, p. 434, Fig Copyright © 2000 The McGraw-Hill Companies. Adapted with permission.)

59
**Section 6.11 The Importance of Fracture Mechanics**

Selection of a Material Design of a Component Design of a Manufacturing or Testing Method Griffith flaw - A crack or flaw in a material that concentrates and magnifies the applied stress.

60
**Example 6.8 Design of a Nondestructive Test**

A large steel plate used in a nuclear reactor has a plane strain fracture toughness of 80,000 psi and is exposed to a stress of 45,000 psi during service. Design a testing or inspection procedure capable of detecting a crack at the edge of the plate before the crack is likely to grow at a catastrophic rate. Example 6.8 SOLUTION

61
**Figure 6.35 Schematic diagram of the Griffith flaw in a ceramic**

(c)2003 Brooks/Cole, a division of Thomson Learning, Inc. Thomson Learning™ is a trademark used herein under license. Figure Schematic diagram of the Griffith flaw in a ceramic

62
**Example 6.9 Properties of SiAlON Ceramics**

Assume that an advanced ceramic, sialon (acronym for SiAlON or silicon aluminum oxynitride), has a tensile strength of 60,000 psi. Let us assume that this value is for a flaw-free ceramic. (In practice, it is almost impossible to produce flaw-free ceramics.) A thin crack 0.01 in. deep is observed before a sialon part is tested. The part unexpectedly fails at a stress of 500 psi by propagation of the crack. Estimate the radius of the crack tip. Example 6.9 SOLUTION

63
**Example 6.10 Design of a Ceramic Support**

Design a supporting 3-in.-wide plate made of sialon, which has a fracture toughness of 9,000 psi , that will withstand a tensile load of 40,000 lb. The part is to be nondestructively tested to assure that no flaws are present that might cause failure. Example 6.10 SOLUTION

64
**Section 6.12 Microstructural Features of Fracture in Metallic Materials**

Transgranular - Meaning across the grains (e.g., a transgranular fracture would be fracture in which cracks would go through the grains). Microvoids - Development of small holes in a material. Intergranular - In between grains or along the grain boundaries. Chevron pattern - A common fracture feature produced by separate crack fronts propagating at different levels in the material.

65
**(c)2003 Brooks/Cole, a division of Thomson Learning, Inc**

(c)2003 Brooks/Cole, a division of Thomson Learning, Inc. Thomson Learning™ is a trademark used herein under license. Figure When a ductile material is pulled in a tensile test, necking begins and voids form – starting near the center of the bar – by nucleation at grain boundaries or inclusions. As deformation continues a 45° shear lip may form, producing a final cup and cone fracture

66
**(c)2003 Brooks/Cole, a division of Thomson Learning, Inc**

(c)2003 Brooks/Cole, a division of Thomson Learning, Inc. Thomson Learning™ is a trademark used herein under license. Figure Dimples form during ductile fracture. Equiaxed dimples form in the center, where microvoids grow. Elongated dimples, pointing toward the origin of failure, form on the shear lip

67
**(c)2003 Brooks/Cole, a division of Thomson Learning, Inc**

(c)2003 Brooks/Cole, a division of Thomson Learning, Inc. Thomson Learning™ is a trademark used herein under license. Figure Scanning electron micrographs of an annealed 1018 steel exhibiting ductile fracture in a tensile test. (a) Equiaxed dimples at the flat center of the cup and cone, and (b) elongated dimples at the shear lip (x 1250)

68
**Example 6.11 Hoist Chain Failure Analysis**

A chain used to hoist heavy loads fails. Examination of the failed link indicates considerable deformation and necking prior to failure. List some of the possible reasons for failure. Example 6.11 SOLUTION 1. The load exceeded the hoisting capacity of the chain. Thus, the stress due to the load exceeded the yield strength of the chain, permitting failure. Comparison of the load to the manufacturer’s specifications will indicate that the chain was not intended for such a heavy load. This is the fault of the user! 2. The chain was of the wrong composition or was improperly heattreated. Consequently, the yield strength was lower than intended by the manufacturer and could not support the load. This may be the fault of the manufacturer!

69
Figure 6.39 Scanning electron micrograph of a brittle fracture surface of a quenched 1010 steel (x 5000). (Courtesy of C.W. Ramsay.)

70
**(c)2003 Brooks/Cole, a division of Thomson Learning, Inc**

(c)2003 Brooks/Cole, a division of Thomson Learning, Inc. Thomson Learning™ is a trademark used herein under license. Figure The Chevron pattern in a 0.5-in.-diameter quenched 4340 steel. The steel failed in a brittle manner by an impact blow

71
**(c)2003 Brooks/Cole, a division of Thomson Learning, Inc**

(c)2003 Brooks/Cole, a division of Thomson Learning, Inc. Thomson Learning™ is a trademark used herein under license. Figure The Chevron pattern forms as the crack propagates from the origin at different levels. The pattern points back to the origin

72
**Example 6.12 Automobile Axle Failure Analysis**

An engineer investigating the cause of an automobile accident finds that the right rear wheel has broken of at the axle. The axle is bent. The fracture surface reveals a Chevron pattern pointing toward the surface of the axle. Suggest a possible cause for the fracture. Example 6.12 SOLUTION The Chevron pattern indicates that the wheel was subjected to an intense impact blow, which was transmitted to the axle, causing failure. Further examination of the fracture surface, microstructure, composition, and properties may verify that the axle was manufactured properly.

73
**Section 6.13 Microstructural Features of Fracture in Ceramics, Glasses, and Composites**

Conchoidal fracture - Fracture surface containing a very smooth mirror zone near the origin of the fracture, with tear lines comprising the remainder of the surface. Delamination - The process by which different layers in a composite will begin to debond.

74
**(c)2003 Brooks/Cole, a division of Thomson Learning, Inc**

(c)2003 Brooks/Cole, a division of Thomson Learning, Inc. Thomson Learning™ is a trademark used herein under license. Figure Scanning electron micrographs of fracture surfaces in ceramics. (a) The fracture surface Al203, showing the cleavage faces (x 1250), and (b) the fracture surface of glass, showing the mirror zone (top) and tear lines characteristic of conchoidal fracture (x 300)

75
**(c)2003 Brooks/Cole, a division of Thomson Learning, Inc**

(c)2003 Brooks/Cole, a division of Thomson Learning, Inc. Thomson Learning™ is a trademark used herein under license. Figure Fiber-reinforced composites can fail by several mechanisms. (a) Due to weak bonding between the matrix and fibers, fibers can pull out of the matrix, creating voids. (b) if the individual layers of the matrix are poorly bonded, the matrix may delaminate, creating voids

76
**Example 6.13 Fracture in Composites**

Describe the difference in fracture mechanism between a boron-reinforced aluminum composite and a glass fiber-reinforced epoxy composite. Example 6.13 SOLUTION In the boron-aluminum composite, the aluminum matrix is soft and ductile; thus we expect the matrix to fail in a ductile manner. Boron fibers, in contrast, fail in a brittle manner. Both glass fibers and epoxy are brittle; thus the composite as a whole should display little evidence of ductile fracture.

77
**Section 6.14 Weibull Statistics for Failure Strength Analysis**

Weibull distribution - A mathematical distribution showing the probability of failure or survival of a material as a function of the stress.

78
**(c)2003 Brooks/Cole, a division of Thomson Learning, Inc**

(c)2003 Brooks/Cole, a division of Thomson Learning, Inc. Thomson Learning™ is a trademark used herein under license. Figure The Weibull distribution describes the fraction of the samples that fail at any given applied stress

79
**Example 6.14 Weibull Modulus for Steel and Alumina Ceramics**

Figure 6.45 shows the log-log plots of the probability of failure and strength of a 0.2% plain carbon steel, an alumina ceramics prepared using conventional powder processing in which alumina powders are compacted in a press and sintered into a dense mass at high temperature. Also, included is a plot for alumina ceramics prepared using special techniques that leads to much more uniform and controlled particle size. This in turn minimizes the flaws. These samples are labeled as controlled particle size (CPS). Comment on the nature of these graphs.

81
Example 6.14 SOLUTION For plain carbon steel the line is almost vertical (i.e., slope or m value is essentially approaching large values). This means that there is very little variation (5 to 10%) in the strength of different samples of the 0.2% C steel. For alumina ceramics prepared using traditional processing, the variability is high (i.e., m is low ~4.7). For ceramics prepared using improved and controlled processing techniques the m is higher ~9.7 indicating a more uniform distribution of flaws. The average strength is also higher (~578 MPa) suggesting lesser number of flaws that will lead to fracture.

82
**Example 6.15 Strength of Ceramics and Probability of Failure**

An advanced engineered ceramic has a Weibull modulus m = 9. The flexural strength is 250 MPa at a probability of failure F = 0.4. What is the level of flexural strength if the probability of failure has to be 0.1?

83
Example 6.15 SOLUTION Equation 6.27 Now, we want to determine the value of for F = 0.1. We know that m = 9 and 0 = MPa, so we need to get the value of . We substitute these values into Equation 6-29:

84
**Example 6.16 Weibull Modulus Parameter Determination**

Seven silicon carbide specimens were tested and the following fracture strengths were obtained: 23, 49, 34, 30, 55, 43, and 40 MPa. Estimate the Weibull modulus for the data by fitting the data to Equation Discuss the reliability of the ceramic. Equation 6.29

85
**(c)2003 Brooks/Cole, a division of Thomson Learning, Inc**

(c)2003 Brooks/Cole, a division of Thomson Learning, Inc. Thomson Learning™ is a trademark used herein under license. Figure Plot of cumulative probability of failure versus fracture stress. Note the fracture strength is plotted on a log scale

86
Example 6.16 SOLUTION

87
Section 6.15 Fatigue Fatigue is the lowering of strength or failure of a material due to repetitive stress which may be above or below the yield strength. Creep - A time dependent, permanent deformation at high temperatures, occurring at constant load or constant stress. Beach or clamshell marks - Patterns often seen on a component subjected to fatigue. Rotating cantilever beam test - An older test for fatigue testing. S-N curve (also known as the Wöhler curve) - A graph showing stress as a function of number of cycles in fatigue.

88
**Figure 6. 47 Fatigue fracture surface**

Figure 6.47 Fatigue fracture surface. (a) At low magnifications, the beach mark pattern indicates fatigue as the fracture mechanism. The arrows show the direction of growth of the crack front, whose origin is at the bottom of the photograph. (Image (a) is from C.C. Cottell, ‘‘Fatigue Failures with Special Reference to Fracture Characteristics,’’ Failure Analysis: The British Engine Technical Reports, American Society for Metals, 1981, p. 318.) (b) At very high magnifications, closely spaced striations formed during fatigue are observed (x 1000)

89
**(c)2003 Brooks/Cole, a division of Thomson Learning, Inc**

(c)2003 Brooks/Cole, a division of Thomson Learning, Inc. Thomson Learning™ is a trademark used herein under license. Figure Schematic representation of a fatigue fracture surface in a steel shaft, showing the initiation region, the propagation of fatigue crack (with beam markings), and catastrophic rupture when the crack length exceeds a critical value at the applied stress

90
**Example 6.17 Fatigue Failure Analysis of a Crankshaft**

A crankshaft in a diesel engine fails. Examination of the crankshaft reveals no plastic deformation. The fracture surface is smooth. In addition, several other cracks appear at other locations in the crankshaft. What type of failure mechanism would you expect? Example 6.17 SOLUTION Since the crankshaft is a rotating part, the surface experiences cyclical loading. We should immediately suspect fatigue. The absence of plastic deformation supports our suspicion. Furthermore, the presence of other cracks is consistent with fatigue; the other cracks didn’t have time to grow to the size that produced catastrophic failure. Examination of the fracture surface will probably reveal beach marks or fatigue striations.

91
**Figure 6.49 Geometry for the rotating cantilever beam specimen setup**

(c)2003 Brooks/Cole, a division of Thomson Learning, Inc. Thomson Learning™ is a trademark used herein under license. Figure Geometry for the rotating cantilever beam specimen setup

92
**(c)2003 Brooks/Cole, a division of Thomson Learning, Inc**

(c)2003 Brooks/Cole, a division of Thomson Learning, Inc. Thomson Learning™ is a trademark used herein under license. Figure The stress-number of cycles to failure (S-N) curves for a tool steel and an aluminum alloy

93
**Section 6.16 Results of the Fatigue Test**

Endurance limit - An older concept that defined a stress below which a material will not fail in a fatigue test. Fatigue life - The number of cycles permitted at a particular stress before a material fails by fatigue. Fatigue strength - The stress required to cause failure by fatigue in a given number of cycles, such as 500 million cycles. Notch sensitivity - Measures the effect of a notch, scratch, or other imperfection on a material’s properties, such as toughness or fatigue life. Shot peening - A process in which metal spheres are shot at a component.

94
**Example 6.18 Design of a Rotating Shaft**

A solid shaft for a cement kiln produced from the tool steel in Figure 6.50 must be 96 in. long and must survive continuous operation for one year with an applied load of 12,500 lb. The shaft makes one revolution per minute during operation. Design a shaft that will satisfy these requirements.

95
**(c)2003 Brooks/Cole, a division of Thomson Learning, Inc**

(c)2003 Brooks/Cole, a division of Thomson Learning, Inc. Thomson Learning™ is a trademark used herein under license. Figure The stress-number of cycles to failure (S-N) curves for a tool steel and an aluminum alloy

96
Example 6.18 SOLUTION

97
**Section 6.17 Application of Fatigue Testing**

(c)2003 Brooks/Cole, a division of Thomson Learning, Inc. Thomson Learning™ is a trademark used herein under license. Figure 6.51 Examples of stress cycles. (a) Equal stress in tension and compression, (b) greater tensile stress than compressive stress, and (c) all of the stress is tensile

98
Figure 6.52 Crack growth rate versus stress-intensity factor range for a high-strength steel. For this steel, C = 1.62 1012 and n = 3.2 for the units shown

99
**Example 6.19 Design of a Fatigue-Resistant Plate**

A high-strength steel plate (Figure 6.52), which has a plane strain fracture toughness of 80 MPa , is alternately loaded in tension to 500 MPa and in compression to 60 MPa. The plate is to survive for 10 years, with the stress being applied at a frequency of once every 5 minutes. Design a manufacturing and testing procedure that assures that the component will serve as intended.

100
Figure 6.52 Crack growth rate versus stress-intensity factor range for a high-strength steel. For this steel, C = 1.62 1012 and n = 3.2 for the units shown

101
Example 6.19 SOLUTION

102
**Section 6.18 Creep, Stress Rupture, and Stress Corrosion**

Stress-rupture curve - A method of reporting the results of a series of creep tests by plotting the applied stress versus the rupture time. Stress-corrosion - A phenomenon in which materials react with corrosive chemicals in the environment leading to the formation of cracks and lowering of strength.

103
**(c)2003 Brooks/Cole, a division of Thomson Learning, Inc**

(c)2003 Brooks/Cole, a division of Thomson Learning, Inc. Thomson Learning™ is a trademark used herein under license. Figure Grain boundary sliding during creep causes (a) the creation of voids at an inclusion trapped at the grain boundary, and (b) the creation of a void at a triple point where three grains are in contact

104
Figure 6.54 Creep cavities formed at grain boundaries in an austentic stainless steel (x 500). (From ASM Handbook, Vol. 7, (1972) ASM International, Materials Park, OH ) Figure 6.55 Photomicrograph of a metal near a stress-corrosion fracture, showing the many intergranular cracks formed as a result of the corrosion process (x 200). (From ASM Handbook, Vol. 7, (1972) ASM International, Materials Park, OH )

105
**Example 6.20 Failure Analysis of a Pipe**

A titanium pipe used to transport a corrosive material at 400oC is found to fail after several months. How would you determine the cause for the failure? Example 6.20 SOLUTION Since a period of time at a high temperature was required before failure occurred, we might first suspect a creep or stress-corrosion mechanism for failure. Microscopic examination of the material near the fracture surface would be advisable. If many tiny, branched cracks leading away from the surface are noted, stress-corrosion is a strong possibility. However, if the grains near the fracture surface are elongated, with many voids between the grains, creep is a more likely culprit.

106
**Section 6.19 Evaluation of Creep Behavior**

Creep test - Measures the resistance of a material to deformation and failure when subjected to a static load below the yield strength at an elevated temperature. Climb - Movement of a dislocation perpendicular to its slip plane by the diffusion of atoms to or from the dislocation line. Creep rate - The rate at which a material deforms when a stress is applied at a high temperature. Rupture time - The time required for a specimen to fail by creep at a particular temperature and stress.

107
**(c)2003 Brooks/Cole, a division of Thomson Learning, Inc**

(c)2003 Brooks/Cole, a division of Thomson Learning, Inc. Thomson Learning™ is a trademark used herein under license. Figure A typical creep curve showing the strain produced as a function of time for a constant stress and temperature

108
**(c)2003 Brooks/Cole, a division of Thomson Learning, Inc**

(c)2003 Brooks/Cole, a division of Thomson Learning, Inc. Thomson Learning™ is a trademark used herein under license. Figure Dislocations can climb (a) when atoms leave the dislocation line to create interstitials or to fill vacancies or (b) when atoms are attached to the dislocation line by creating vacancies or eliminating interstitials

109
**(c)2003 Brooks/Cole, a division of Thomson Learning, Inc**

(c)2003 Brooks/Cole, a division of Thomson Learning, Inc. Thomson Learning™ is a trademark used herein under license. Figure The effect of temperature or applied stress on the creep curve

110
**Section 6.20 Use of Creep Data**

Stress-rupture curve - A method of reporting the results of a series of creep tests by plotting the applied stress versus the rupture time. Larson-Miller parameter - A parameter used to relate the stress, temperature, and rupture time in creep.

111
**(c)2003 Brooks/Cole, a division of Thomson Learning, Inc**

(c)2003 Brooks/Cole, a division of Thomson Learning, Inc. Thomson Learning™ is a trademark used herein under license. Figure 6.59 Results from a series of creep tests. (a) Stress-rupture curves for an iron-chromium-nickel alloy and (b) the Larson-Miller parameter for ductile cast iron

112
**Example 6.21 Design of Links for a Chain**

Design a ductile cast iron chain (Figure 6.60) to operate in a furnace used to fire ceramic bricks. The furnace is to operate without rupturing for five years at 600oC, with an applied load of 5000 lbs. (c)2003 Brooks/Cole, a division of Thomson Learning, Inc. Thomson Learning™ is a trademark used herein under license. Figure Sketch of chain link (for Example 6.21)

113
Example 6.21 SOLUTION

114
**Section 6.21 Superplasticity**

Superplasticity - Large deformations in materials, resulting from high temperatures and low strain rates.

115
**(c)2003 Brooks/Cole, a division of Thomson Learning, Inc**

(c)2003 Brooks/Cole, a division of Thomson Learning, Inc. Thomson Learning™ is a trademark used herein under license. Figure The S-N fatigue curve for an acetal polymer (for Problems 6.87, 6.89, and 6.90)

116
**(c)2003 Brooks/Cole, a division of Thomson Learning, Inc**

(c)2003 Brooks/Cole, a division of Thomson Learning, Inc. Thomson Learning™ is a trademark used herein under license. Figure The crack growth rate for an acrylic polymer (for Problems 6.93, 6.94, 6.95)

117
**Figure 6.63 Hook (For Problem 6.113)**

(c)2003 Brooks/Cole, a division of Thomson Learning, Inc. Thomson Learning™ is a trademark used herein under license. Figure Hook (For Problem 6.113)

118
**(c)2003 Brooks/Cole, a division of Thomson Learning, Inc**

(c)2003 Brooks/Cole, a division of Thomson Learning, Inc. Thomson Learning™ is a trademark used herein under license. Figure (Repeated for Problems 6.86, and 6.88) The stress-number of cycles to failure (S-N) curves for a tool steel and an aluminum alloy

119
**(c)2003 Brooks/Cole, a division of Thomson Learning, Inc**

(c)2003 Brooks/Cole, a division of Thomson Learning, Inc. Thomson Learning™ is a trademark used herein under license. Figure 6.52 (Repeated for Problems 6.91 and 6.92) Crack growth rate versus stress-intensity factor range for a high-strength steel. For this steel, C = 1.62 x 10 –12 and n = 3.2 for the units shown

120
**(c)2003 Brooks/Cole, a division of Thomson Learning, Inc**

(c)2003 Brooks/Cole, a division of Thomson Learning, Inc. Thomson Learning™ is a trademark used herein under license. Figure 6.59 (Repeated for Problems through 6.112) Results from a series of creep tests. (a) Stress-rupture curves for an iron-chromium-nickel alloy and (b) the Larson-Miller parameter for ductile cast iron

Similar presentations

Presentation is loading. Please wait....

OK

Mechanical Properties of Materials

Mechanical Properties of Materials

© 2017 SlidePlayer.com Inc.

All rights reserved.

Ads by Google

Ppt on tools of data collection Ppt on area related to circles for class 10 Ppt on astronomy and astrophysics major Ppt on different festivals of india Ppt on cartesian product database Ppt on exploring fibonacci numbers Ppt on do's and don'ts of group discussion games Ppt on leadership Ppt on indo islamic architecture Ppt on dc series motor